Synthesis and Theoretical Investigations of the Solid Solution CeRu1-xNixAl (x = 0.1-0.95) Showing Cerium Valence Fluctuations.
Niehaus, Oliver; Rodewald, Ute Ch; Abdala, Paula M.; Touzani, Rachid St; Fokwa, Boniface P. T.; Janka, Oliver; Inorganic chemistry 53 (2014) 2471–2480; doi:10.1021/ic402414f

data_4337828
_publ_section_title
;
 Synthesis and Theoretical Investigations of the Solid Solution
 CeRu1-xNixAl (x = 0.1-0.95) Showing Cerium Valence Fluctuations.
;
_journal_issue                   5
_journal_name_full               'Inorganic chemistry'
_journal_page_first              2471
_journal_page_last               2480
_journal_paper_doi               10.1021/ic402414f
_journal_volume                  53
_journal_year                    2014
_chemical_formula_sum            'Al Ce Ni0.3 Ru0.7'
_chemical_formula_weight         255.36
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   7.0835(3)
_cell_length_b                   4.1384(2)
_cell_length_c                   15.7571(8)
_cell_measurement_temperature    293(2)
_cell_volume                     461.91(4)
_computing_cell_refinement       'IPDS package'
_computing_data_collection       'IPDS package'
_computing_data_reduction        'IPDS package'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'STOE IPDS-II'
_diffrn_measurement_method       'oscillation mode'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0540
_diffrn_reflns_av_sigmaI/netI    0.0265
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            13357
_diffrn_reflns_theta_full        34.84
_diffrn_reflns_theta_max         34.84
_diffrn_reflns_theta_min         3.15
_exptl_absorpt_coefficient_mu    26.4
_exptl_absorpt_correction_T_max  0.560
_exptl_absorpt_correction_T_min  0.206
_exptl_absorpt_correction_type   numerical
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    7.34
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             881
_exptl_crystal_size_max          0.060
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.040
_refine_diff_density_max         1.291
_refine_diff_density_min         -1.750
_refine_diff_density_rms         0.342
_refine_ls_extinction_coef       0.00139(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.104
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_reflns         1117
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.104
_refine_ls_R_factor_all          0.0366
_refine_ls_R_factor_gt           0.0265
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0128P)^2^+3.9337P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0507
_refine_ls_wR_factor_ref         0.0521
_reflns_number_gt                926
_reflns_number_total             1117
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic402414f_si_002.cif
_cod_data_source_block           CeRu0.7Ni0.3Al
_cod_original_sg_symbol_H-M      Pnma
_cod_original_formula_sum        'Al Ce Ni0.30 Ru0.70'
_cod_database_code               4337828